ARTICLE IN PRESS
Solar Energy Materials & Solar Cells 91 (2007) 1388–1391 www.elsevier.com/locate/solmat
Bifacial conﬁgurations for CdTe solar cells A. Romeob,, G. Khrypunovc, S. Galassinid, H. Zogga, A.N. Tiwaria,e a
Thin Film Physics Group, Laboratory for Solid State Physics, ETH, Swiss Federal Institute of Technology, Zu¨rich, Technoparkstrasse 1, 8005 Zurich, Switzerland b Scientific and Technological Department, University of Verona, Ca’ Vignal 2, Strada Delle Grazie 15, 37134 Verona, Italy c National Technical University, 61002 Kharkov, Ukraine d Medicine and Public Health Department, University of Verona, Ca’ Vignal 2, Strada Delle Grazie, 37134 Verona, Italy e Department of Electronic and Electrical Engineering, Centre for Renewable Energy Systems and Technology (CREST), Loughborough University, Leicestershire LE11 3TU, UK Available online 9 May 2007
Abstract We present a different back contact for CdTe solar cell by the application of only a transparent conducting oxide (TCO), typically ITO, as a back electrical contact on all-PVD CdTe/CdS photovoltaic devices that acts as a free-Cu stable back contact and at the same time allows to realize bifacial CdTe solar cells, which can be illuminated from either or both sides. Also devices with thin CdTe layers (from 2 mm down to 1 mm) have been prepared to improve the conversion efﬁciency on the back side illumination, which is limited by the collection of carriers far away from the junction and to reduce the amount of material in the CdTe device. Reproducible solar cells exceeding 10% efﬁciency on the front side illumination and exceeding 3% on the back side illumination are reported. r 2007 Elsevier B.V. All rights reserved. Keywords: Thin ﬁlms; CdTe; Bifacial cells
1. Introduction The CdTe thin ﬁlm solar cells have now established longterm stable performance , high efﬁciency up to 16.5% under AM1.5 illumination  and easy scale-up for largearea production . High efﬁciency and fast deposition for CdTe by close space sublimation (CSS) allows high throughput and potentially cheap in-line production of solar modules. In order to improve the efﬁciency of photovoltaic cells by preparing tandem cells, bifacial conﬁguration thin ﬁlm devices have been introduced from the early 1980s up to our days [4,5]. For CdTe solar cells inserting a transparent back contact is a particularly challenging task because of both the high electron afﬁnity and high-energy band gap of CdTe [6,7]. Some groups have faced this problem introducing CuTe  or ZnTe . We have introduced a different approach to apply a transparent back contact on CdTe solar cells: a thin layer Corresponding author. Tel.: +390458027974; fax: +390458027051.
E-mail address: [email protected]
(A. Romeo). 0927-0248/$ - see front matter r 2007 Elsevier B.V. All rights reserved. doi:10.1016/j.solmat.2007.03.010
of transparent and conducting ITO . Due to the transparency of the ITO back contact and FTO front contact, solar cells can be illuminated both from the front and rear sides like a bifacial solar cell . Previously a preliminary development of this back contact has been presented, a promising efﬁciency of about 9% and proved stability for these solar cells has been developed . Our CdTe/CdS fabrication process has been already presented. Brieﬂy all the layers are grown by PVD methods using tin oxide-doped with ﬂuorine (FTO) as front contact and copper–gold layer as back contact . Standard solar cells have a typical efﬁciency range of 11–12.5% [6,13].
2. Copper-free bifacial cells ITO back contact has been applied by RF sputtering after a bromine methanol etching: the layer has a sufﬁcient transparency, more than 85%, together with a good conductivity about 10 O/square. As deposited solar cells with pure ITO back contact perform typically very low
ARTICLE IN PRESS A. Romeo et al. / Solar Energy Materials & Solar Cells 91 (2007) 1388–1391
efﬁciencies around 2.5% in particular Voc and ﬁll factor are poor, respectively, around 350 mV and 35%. However, we applied an annealing treatment to the ITO back contacted CdTe cells: different cells have been prepared and after ITO RF-sputtering, annealing in air has been provided at different temperatures from 200 up to 400 1C; best results were given with annealing around 350 1C. The results are that from a starting efﬁciency of 1–2% after light soaking and annealing, it jumps to 4–5% that can still raise to an upper efﬁciency above 6% under light soaking. If we analyse the standard Cu/Au contact, we can observe that the efﬁciency of the solar cells jumps from a poor efﬁciency up to 10% efﬁciency after postdeposition annealing treatment As previously shown , the interesting feature of these solar cells is the stability under accelerated lifetime test. We have performed preliminary test also on these devices (solar cells were kept under 1 sun illumination and at 80 1C temperature in open circuit conditions) and they presented an excellent stability and the performance actually improves instead of degrading (see Fig. 1). The light soaking effect is different in case of asdeposited and annealed devices: in the as deposited device the improvement is very high in the ﬁrst days (from about 1% efﬁciency up to above 3% efﬁciency) and successively tends to stabilize. In the annealed devices, the improvement is lower but still there is a constant increase in an almost 10 years estimated working time. The defects at the junction between the ITO and the CdTe are more in the as-deposited case and the light soaking ﬁlls the recombination centres at the junction while in case of the annealed device the hetero-junction presents a better intermixing and probably the crystallised Te layer helps to inject the carriers across the junction.
3. Copper-containing bifacial cells In order to compare the ITO-back-contacted cells with the standard copper–gold ones, we have analysed the possibility of inserting copper in the back contact and to study the effects in the performance and in the stability. The basic principle is that a small amount of copper would still leave the back contact transparent and at the same time might not affect the stability of the solar cell. Prior to the copper deposition, a standard bromine– methanol etching is applied and after copper deposition by physical vapour, the ITO layer is deposited by RF sputtering as previously presented. Several different devices have been made with a standard fabrication process but with different quantities of copper. In Fig. 1, accelerated lifetime stability tests of cells with different amount of copper are shown. Both start with very similar efﬁciency but the stability trend is opposite. The 3-nm-Cu cell has a degradation that tends to stabilize after 4 years estimated time, on the other hand the o0.5 nm-Cu cell (we believe that at such low quantity of copper, the quartz is not as precise that is the reason why we have put an indicative number of less than 0.5 nm, more investigations on this has to be done) starts from the same efﬁciency but instead of degrading it improves slightly in the performance. The behaviour of the 3-nm-Cu cell is similar to the one observed for Cu/Au  but still the stability is higher. In the back side illumination, the solar cells perform efﬁciencies in the order of 0.5% with Voc of about 300 mV, Jsc of 3–4 mA/cm2 and ﬁll factor of 45%. The low current in the back side illumination is due to the long distance between the hole–electron pair generation and the junction.
Fig. 1. Accelerated lifetime stability tests of an ITO/CdTe/CdS/FTO solar cell: before (A) and after annealing at 350 1C (B) and of ITO/Cu/CdTe/CdS/ FTO solar cells with 3 nm copper deposition (C) and less than 0.5 nm copper deposition (D).
ARTICLE IN PRESS 1390
A. Romeo et al. / Solar Energy Materials & Solar Cells 91 (2007) 1388–1391
However, the o0.5 nm-Cu cell has a very similar behaviour of Sb2Te3/Mo cell  with a rapid increase at the beginning of the light soaking and a successive stabilization, suggesting that the copper gives instability only if the back contact is not well designed. We believe that if a stable compound with Cu is formed, then the back contact could be very stable: in particular, what could happen is that after the creation of a thin layer of tellurium due to the bromine–methanol etching the copper reacts with the tellurium giving place to copper telluride which is a stable compound. Quantum efﬁciency measurements, not shown here, have been made and the results have been compared with the one of the standard Cu/Au contacted cell. The latter has a very similar response in the red part near the absorption edge, but has a better response in the 400–550 nm region most probably due to the presence of copper in the bulk of CdTe which passivates the grain boundaries increasing the quantum efﬁciency . This is an indirect proof that copper is not penetrating in the CdTe layer if the amount is low enough to bind with free Te. The proof for stability comes also from the annealing test made successively on the light soaked cells, annealing on these devices has been performed for 25 min at 300 1C. The annealed cells did not degrade but instead their efﬁciency improved in general of about 20%. The increase of the efﬁciency could be interpreted with the re-crystallization of the CuxTe1–x layer, which increases the conductivity of the back contact, but more investigations have to be done.
Fig. 2. Front (A) (Voc ¼ 710 mV, Jsc ¼ 19.4 mA/cmA2, FF ¼ 74.6%, Z ¼ 10.3%) and back (B) illuminated (Voc ¼ 659 mV, Jsc ¼ 8.8 mA/ cmA2, FF ¼ 36%, Z ¼ 2.1%) CdTe solar cell with 2.5-mm-thick absorber.
4. Thin absorber bifacial cells In order to improve the performance in the back side illumination, we reduced the thickness of CdTe. The solar cell fabrication process has been adjusted to the different CdTe thickness; in particular the CdCl2 treatment has been processed with only 20% of the standard CdCl2 quantity and by reducing the annealing time. The ﬁrst cells were made with about 2.5 mm CdTe thickness and the optimized quantity of copper (less than 0.5 nm). The solar cells started with a very good performance from the beginning (9.5%) and increased after light soaking to reach an efﬁciency exceeding 10% as shown in Fig. 2. The back side illumination performance improved considerably compared to the standard cell. As shown in Fig. 2, after 3 days light soaking we have 2.1%. Accelerated lifetime stability test have been provided: the cells are practically stable having a strong increase at the beginning and a successive short degradation afterwards. A further reduction of the CdTe thickness could open up different possibilities: a further increase in the back side illumination performance, application for tandem conﬁguration cells and a mirror on top could be applied in order to absorb all the light with a very low amount of material used. One micron CdTe thick solar cells have been
Fig. 3. Front (A) (Voc ¼ 676 mV, Jsc ¼ 19.7 mA/cm2, FF ¼ 60.5%, Z ¼ 8%) and back (B) illuminated (Voc ¼ 622 mV, Jsc ¼ 12.2 mA/cm2, FF ¼ 43%, Z ¼ 3.2%) CdTe solar cell with 1-mm-thick absorber.
prepared using a reduced CdCl2 treatment, 30 nm thick CdCl2 and 15 min annealing in air at standard annealing temperatures, copper insertion has been reduced to less than 0.3 nm. As expected, the current density is reduced and the overall efﬁciency drops to 7–8%, however, the performance in the back side illumination improves up to more than 3% (see Fig. 3). The maximum efﬁciency is obtained after some days under light soaking and then there is a slight degradation, similar to the behaviour shown in Fig. 1 for the thicker cell. 5. Conclusions Application of a different back contact, based on TCO, on p-CdTe opens a variety of new applications of CdTe solar cells. They can work as bifacial cells, illuminating the back and the front surfaces simultaneously or they can be used in tandem solar cells. The controlled insertion of a very limited amount of copper into the ITO back contact permits to have reproducible devices with high efﬁciencies still keeping the bifacial conﬁguration.
ARTICLE IN PRESS A. Romeo et al. / Solar Energy Materials & Solar Cells 91 (2007) 1388–1391
Thin CdTe layer solar cells have been realized with efﬁciencies exceeding 10%. The reduced thickness of CdTe allows to have a better performance (efﬁciencies exceeding 3.5%) on the back side illumination and reduces the amount of CdTe material increasing the transparency. Solar cell layers need further optimisation and transport properties need investigation to improve the efﬁciency of bifacial cells. However, TCO back contact on CdTe provides superior cell stability, simpliﬁed processing and a potential for low-cost production. Acknowledgements The Italian Ministry of Research and the Swiss National Foundation (Project SCOPES IB 7420-111038) are thankfully acknowledged. References  D.L. Batzner, A. Romeo, H. Zogg, R. Wendt, A.N. Tiwari, Thin Solid Films 387 (2001) 151.  X. Wu, J. C. Keane, R. G. Dhere, C. DeHart, D. S. Albin, A. Duda, T. A. Gessert, S. Asher, D. H. Levi, P. Sheldon, in: Proceedings of 17th European Photovoltaic Solar Energy Conference, Munich, Germany, 2001, p. 995.
 A. Abken, C. Hambro, P. Meyers, R. Powell, S. Zafar, in: NCPV and Solar Program Review Meeting, NREL, USA, 2003, p. 393.  P.V. Meyers, C.H. Liu, L Russell, V. Ramanathan, R.W. Birkmire, B.E. McCandless, J.E. Phillips, in: Proceedings of the 20th IEEE Photovoltaic Specialists Conference, 1988, p. 1448.  T. Nakada, Y. Hirabayashi, T. Tokado, D. Ohmori, T. Mise, Sol. Energy 77 (2004) 739–747.  A. Romeo, M. Terheggen, D. Abou-Ras, D.L. Ba¨tzner, F.-J. Haug, M. Ka¨lin, D. Rudmann, A.N. Tiwari, Res. Appl. 12 (2–3) (2004) 93.  D. Desai, S.S. Hegedus, B.E. McCandless, R.W. Birkmire, K.D. Dobson, D. Ryan, in: Proceedings of WCPEC-4, Hawaii, 2006.  X. Wu, J. Zhou, A. Duda, J.C. Keane, T.A. Gessert, Y. Yan, R. Nouﬁ, Res. Appl. 14 (2006) 471.  D. Desai, S.S. Hegedus, B.E. McCandless, D. Ryan, Thin-ﬁlm compound semiconductor photovoltaics, in: W. Shafarman, T. Gessert, S. Niki, S. Siebentritt (Eds.), Material Research Society Sympsium Proceedings, Warrendale, PA, vol. 865, 2005 p. F14.9  A.N. Tiwari, G. Khrypunov, F. Kurdzesau, D.L. Ba¨tzner, A. Romeo, H. Zogg, Progress in photovoltaics, Res. Appl. 12 (2004) 33.  G. Khrypunov, A. Romeo, F. Kurdesau, D.L. Baetzner, H. Zogg, A.N. Tiwari, Sol. Energy Mater. Sol. Cells 90 (2006) 664.  D.L. Ba¨tzner, A. Romeo, H. Zogg, A.N. Tiwari, in: Proceedings of the 16th European Photovoltaic Solar Energy Conference and Exhibition, Glasgow, Scotland, 2000, p. 353.  A. Romeo, H. Zogg, A. N. Tiwari, in: Proceedings of Second World Conference and Exhibition on Photovoltaic Solar Energy Conversion, Vienna, Austria, 1998, p. 1105.  D. Bonnet, P. Meyer, J. Mater. Res. 13 (10) (1998) 2740.